Solvothermal syntheses, structures, and magnetic properties of three cobalt coordination polymers constructed from naphthalene-1,4-dicarboxylic acid and bis(imidazole) linkers
Dong, Jun-Liang; He, Kun-Huan; Wang, Duo-Zhi; Zhang, Ying-Hui; Wang, Dan-Hong; Journal of Solid State Chemistry 263 (2018) 164–171; doi:10.1016/j.jssc.2018.04.019

data_1561060
_publ_section_title
;
 Solvothermal syntheses, structures, and magnetic properties of three
 cobalt coordination polymers constructed from
 naphthalene-1,4-dicarboxylic acid and bis(imidazole) linkers
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              164
_journal_page_last               171
_journal_paper_doi               10.1016/j.jssc.2018.04.019
_journal_volume                  263
_journal_year                    2018
_chemical_formula_moiety         '0.5(C100 H68 Co6 N16 O24)'
_chemical_formula_sum            'C50 H34 Co3 N8 O12'
_chemical_formula_weight         1115.64
_space_group_crystal_system      monoclinic
_space_group_IT_number           15
_space_group_name_Hall           '-C 2yc'
_space_group_name_H-M_alt        'C 1 2/c 1'
_atom_sites_solution_hydrogens   geom
_cell_angle_alpha                90
_cell_angle_beta                 91.27(3)
_cell_angle_gamma                90
_cell_formula_units_Z            4
_cell_length_a                   22.634(4)
_cell_length_b                   10.384(2)
_cell_length_c                   22.097(4)
_cell_measurement_reflns_used    4360
_cell_measurement_temperature    293(2)
_cell_measurement_theta_max      0.825
_cell_measurement_theta_min      0.808
_cell_volume                     5192.2(17)
_computing_molecular_graphics    'Olex2 (Dolomanov et al., 2009)'
_computing_publication_material  'Olex2 (Dolomanov et al., 2009)'
_computing_structure_refinement  'XL (Sheldrick, 2008)'
_diffrn_ambient_temperature      293(2)
_diffrn_measured_fraction_theta_full 0.998
_diffrn_measured_fraction_theta_max 0.995
_diffrn_measurement_device_type  CCD
_diffrn_measurement_method       '\w scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0899
_diffrn_reflns_av_unetI/netI     0.0756
_diffrn_reflns_Laue_measured_fraction_full 0.998
_diffrn_reflns_Laue_measured_fraction_max 0.995
_diffrn_reflns_limit_h_max       29
_diffrn_reflns_limit_h_min       -29
_diffrn_reflns_limit_k_max       13
_diffrn_reflns_limit_k_min       -13
_diffrn_reflns_limit_l_max       28
_diffrn_reflns_limit_l_min       -28
_diffrn_reflns_number            26269
_diffrn_reflns_point_group_measured_fraction_full 0.998
_diffrn_reflns_point_group_measured_fraction_max 0.995
_diffrn_reflns_theta_full        25.242
_diffrn_reflns_theta_max         27.475
_diffrn_reflns_theta_min         3.338
_exptl_absorpt_coefficient_mu    1.015
_exptl_absorpt_correction_type   none
_exptl_crystal_colour            red
_exptl_crystal_density_diffrn    1.427
_exptl_crystal_description       block
_exptl_crystal_F_000             2268
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.2
_exptl_crystal_size_min          0.19
_platon_squeeze_details
;
TITL 1 in C2/c New: C2/c
CELL   22.6340   10.3840   22.0970     90.00     91.27     90.00
SPGR C2/c
Q101 0.710 0.277 0.045 !       4.63 eA-3
Q102 0.733 0.217 0.958 !       4.51 eA-3
Q103 0.367 0.342 0.387 !       4.36 eA-3
C104 0.156 0.255 0.529 !       4.26 eA-3
Q105 0.819 0.344 0.065 !       4.08 eA-3
Q106 0.318 0.187 0.541 !       3.67 eA-3
C107 0.111 0.319 0.495 !       3.21 eA-3
C108 0.873 0.335 0.064 !       3.20 eA-3
C109 0.970 0.087 0.954 !       3.14 eA-3
Q110 0.319 0.313 0.388 !       2.49 eA-3
Q111 0.156 0.415 0.427 !       1.35 eA-3
Q112 0.164 0.433 0.273 !       1.29 eA-3
Q113 0.955 0.188 0.380 !       1.25 eA-3
Q114 0.165 0.464 0.234 !       1.22 eA-3
Q115 1.000 0.469 0.249 !       1.20 eA-3
Q116 0.639 0.124 0.820 !       1.18 eA-3
Q117 0.876 0.190 0.927 !       1.16 eA-3
Q118 0.829 0.192 0.790 !       1.15 eA-3
Q119 0.719 0.110 0.969 !       1.12 eA-3
Q120 0.805 0.061 0.756 !       1.11 eA-3
Q121 0.682 0.130 0.786 !       1.11 eA-3
Q122 0.390 0.030 0.457 !       1.10 eA-3
Q123 0.563 0.376 0.108 !       1.08 eA-3
Q124 0.038 0.255 0.874 !       1.08 eA-3
C125 0.439 0.347 0.485 !       1.06 eA-3
C126 0.939 0.847 0.485 !       1.06 eA-3
Q127 0.282 0.312 0.817 !       1.06 eA-3
C128 0.147 0.340 0.536 !       1.05 eA-3
Q129 0.343 0.507 0.643 !       1.04 eA-3
Q130 0.618 0.271 0.938 !       1.04 eA-3
C131 0.109 0.278 0.472 !       1.03 eA-3
Q132 0.545 0.441 0.579 !       1.01 eA-3
Q133 0.463 0.383 0.406 !       1.00 eA-3
Q134 0.695 0.089 0.049 !       0.98 eA-3
Q135 0.991 0.508 0.966 !       0.97 eA-3
Q136 0.188 0.057 0.491 !       0.97 eA-3
Q137 0.641 0.034 0.209 !       0.97 eA-3
Q138 0.806 0.369 0.335 !       0.97 eA-3
Q139 0.306 0.869 0.335 !       0.97 eA-3
Q140 0.688 0.255 0.249 !       0.96 eA-3
Q141 0.245 0.284 0.112 !       0.96 eA-3
Q142 0.921 0.039 0.667 !       0.95 eA-3
Q143 0.588 0.505 0.571 !       0.95 eA-3
Q144 0.025 0.435 0.062 !       0.95 eA-3
Q145 0.306 0.441 0.576 !       0.94 eA-3
Q146 0.573 0.346 0.311 !       0.94 eA-3
Q147 0.476 0.406 0.124 !       0.93 eA-3
Q148 0.990 0.411 0.039 !       0.93 eA-3
Q149 0.773 0.405 0.279 !       0.93 eA-3
Q150 0.210 0.441 0.262 !       0.93 eA-3
Q151 0.500 0.339 0.225 !       0.93 eA-3
Q152 0.587 0.325 0.145 !       0.92 eA-3
Q153 0.477 0.504 0.522 !       0.91 eA-3
Q154 0.969 0.128 0.457 !       0.91 eA-3
Q155 0.876 0.060 0.046 !       0.91 eA-3
Q156 0.658 0.052 0.014 !       0.91 eA-3
Q157 0.494 0.558 0.579 !       0.91 eA-3
Q158 0.994 0.058 0.579 !       0.91 eA-3
Q159 0.546 0.474 0.561 !       0.91 eA-3
Q160 0.983 0.027 0.338 !       0.90 eA-3
C161 0.578 0.347 0.070 !       0.90 eA-3
Q162 0.117 0.410 0.508 !       0.90 eA-3
Q163 0.017 0.371 0.605 !       0.90 eA-3
Q164 0.162 0.436 0.653 !       0.90 eA-3
Q165 0.307 0.460 0.394 !       0.89 eA-3
Q166 0.431 0.477 0.493 !       0.89 eA-3
Q167 0.343 0.311 0.265 !       0.89 eA-3
Q168 0.974 0.467 0.674 !       0.89 eA-3
Q169 1.000 0.438 0.752 !       0.89 eA-3
Q170 0.538 0.086 0.145 !       0.89 eA-3
Q171 0.397 0.400 0.434 !       0.88 eA-3
Q172 0.858 0.336 0.112 !       0.88 eA-3
Q173 0.054 0.220 0.330 !       0.88 eA-3
Q174 0.180 0.367 0.334 !       0.88 eA-3
Q175 0.139 0.340 0.294 !       0.88 eA-3
C176 0.022 0.034 0.017 !       0.88 eA-3
Q177 0.542 0.199 0.845 !       0.88 eA-3
Q178 0.984 0.065 0.020 !       0.88 eA-3
Q179 0.478 0.097 0.197 !       0.87 eA-3
Q180 0.712 0.185 0.423 !       0.87 eA-3
Q181 0.680 0.307 0.365 !       0.86 eA-3
Q182 0.522 0.034 0.300 !       0.86 eA-3
Q183 0.427 0.127 0.574 !       0.86 eA-3
Q184 0.643 0.446 0.780 !       0.86 eA-3
Q185 0.033 0.153 0.742 !       0.85 eA-3
Q186 0.031 0.182 0.638 !       0.85 eA-3
Q187 0.531 0.161 0.560 !       0.85 eA-3
Q188 0.842 0.430 0.947 !       0.85 eA-3
Q189 0.837 0.160 0.932 !       0.85 eA-3
Q190 0.062 0.199 0.604 !       0.85 eA-3
Q191 0.235 0.068 0.497 !       0.85 eA-3
Q192 0.969 0.651 0.935 !       0.84 eA-3
Q193 0.492 0.119 0.747 !       0.84 eA-3
Q194 0.008 0.178 0.683 !       0.84 eA-3
Q195 0.445 0.432 0.356 !       0.84 eA-3
Q196 0.616 0.071 0.405 !       0.84 eA-3
Q197 0.494 0.247 0.082 !       0.82 eA-3
Q198 0.156 0.125 0.697 !       0.82 eA-3
Q199 0.252 0.402 0.295 !       0.82 eA-3
;
_refine_diff_density_max         2.488
_refine_diff_density_min         -1.374
_refine_diff_density_rms         0.181
_refine_ls_extinction_coef       .
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.165
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     330
_refine_ls_number_reflns         5928
_refine_ls_number_restraints     27
_refine_ls_restrained_S_all      1.177
_refine_ls_R_factor_all          0.1675
_refine_ls_R_factor_gt           0.0744
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.1052P)^2^+177.8875P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.3222
_refine_ls_wR_factor_ref         0.3390
_reflns_Friedel_coverage         0.000
_reflns_Friedel_fraction_full    .
_reflns_Friedel_fraction_max     .
_reflns_number_gt                4360
_reflns_number_total             5928
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            JSSC-2018-263-164.cif
_cod_data_source_block           2
_cod_database_code               1561060
_shelx_estimated_absorpt_t_max   0.831
_shelx_estimated_absorpt_t_min   0.815
_olex2_refinement_description
;
1. Fixed Uiso
 At 1.2 times of:
  All C(H) groups
2. Restrained distances
 C25-O6
 1.25 with sigma of 0.02
 O5-C25
 1.45 with sigma of 0.02
3. Rigid bond restraints
 C25, O5
 with sigma for 1-2 distances of 0.01 and sigma for 1-3 distances of 0.02
4. Uiso/Uaniso restraints and constraints
Uanis(C25) \\sim Ueq: with sigma of 0.01 and sigma for terminal atoms of 0.02
Uanis(O5) \\sim Ueq: with sigma of 0.005 and sigma for terminal atoms of 0.01
Uanis(C22) \\sim Ueq, Uanis(C21) \\sim Ueq: with sigma of 0.01 and sigma for
terminal atoms of 0.02
5.a Aromatic/amide H refined with riding coordinates:
 C1(H1), C2(H2), C3(H3), C4(H4), C5(H5), C7(H7), C8(H8), C10(H10), C11(H11),
 C12(H12), C15(H15), C16(H16), C20(H20), C23(H23), C21(H21), C22(H22), C25(H25)
;
_platon_squeeze_void_probe_radius 1.20